How to process laminated glass with eva film interlayer successfully
How to Process Laminated Glass with EVA Film InterlayerBy Peter LinHow Do You Process Laminated Glass with EVA Film?1)Processing the Laminated Glass with EVA Film is different from the laminating with PVBFilm.Different in Oven: Laminating with PVB Film you need autoclave; laminating with EVA Film youneed a simple oven: one-step laminating oven which is simpler and easier to process, and lesscost to install.2)Install the ONE-Step of vacuum laminating OvenMake sure the siliconee vacuuming bag is great, and the heating is even inside the oven.3)Combine the pre-laminated glassNormal the combination is :GLASS+EVA FILM+GLASSCut the extra EVA Film gently.Solid the pre-laminated glass with high-temperature green ribbon tape4) Put the pre-laminated glass inside siliconee vacuum bagSeal the siliconee vacuum bag.Start vacuum pump, double check the vacuuming is working well, and the value of vacuum pumpreaches the requirement.5)Heating in two temperature stagesNormally, the heating will be set in two stage:Low temperature stage: 60 degrees C for 15 minutesHigh temperature stage:130 degrees C for 40 minutes6)Do NOT stop vacuuming after the laminated glass is cool as room temperatureDon’t stop vacuuming until the laminated glass is cool to the room temperature, Or the bubbleswill come out inside the laminated glass.Preparation for Glass Lamination with EVA FilmPreparation for Lamination:1)Cut the glass as the size you want, and use Glass Edging Machines to shape the edges of theglasses, which will avoid the glasses hurt the silicone vacuum bag.
2)Use the purified water, deionized water, industrial alcohol or Ethanol to clean the glasses, thenuse the clean hot wind to dry the glasses. Make sure no black spot, water mark, finger print etcon the glasses.Pre-Laminating:1)Put the EVA FILM on the bottom glass, make sure the EVA Film is plain, then put the otherglass on the EVA Film, then use the high-temperature-resistance green ribbon tape to solid thepre-laminated glass.2)Cut the extra EVA FILM that outside the pre-laminated glass. Don’t pull the EVA Film hard toavoid the remove of the EVA Film. Cutting out the extra EVA Film can void the extra EVA Filmmelting and sealing the edges of the laminating glass and hold back vacuuming.3)When you put the pre-laminated glass in the siliconee bag, make sure that each pre-laminatedglass is 3-5cm away from each other to help vacuuming.4)To help vacuuming, you can also put the wooden bar around the silicone bag to helpvacuuming.Notes: if you seal the pre-laminated glass totally with tape, you need to make some small holeson the tapes to help vacuuming.Heating Procedures of Laminating Glass with EVA Film1)Before the silicone bag shelf being pushed into the oven, start the vacuum pump to vacuumingfor 3-5 minutes. Check whether the silicone bag is leaking or not. And the vacuum value shouldat least be 0.095Mpa.2)Push the silicone bag shelf into the oven, then set the parameters of temperature and time.Following two STAGE heating temperature and time. The low temperature stage is 60degress Cand 15mins. And the high temperature stage is 130 degree C and 40 mins (notes:following theinstructions that the EVA FILM MANUFACTURERS give to you, the parameters maybe different
for different manufacturers). Because it takes time for the heat transfer through the silicone bag,so the temperature the detector gets may be different from the real temperature of the laminatedglass.3)Stop heating. Wait till the temperature is lower than 75 degrees, then open the oven door andpull out the silicone shelf to help cooling. But don’t open the silicone bag or let cold water touchthe laminated glass.4)After the temperature is lower than 45 degree, now you can open the silicone bag and checkthe laminated glass.Processing Temperature and Time for Laminating Glass with EVA FILMFirst I would to say that no fixed standard value for the processing parameters, because differentEVA film manufacturer have different formula for the EVA FILM, and different glass laminatingmachine manufacturer have different property for the machine.What’s more, the weather andmoisture is different in different regions, which also would affect the processing parameters. Sothere is no fixed standard value for the processing temperature and time for laminating glass withEVA FILM.But I can tell you some general rules of the processing parameters for laminating glass with EVAFILM.1) Indoor EVA FILM (like 110 degrees C) need lower temperature for laminating than outdoorEVA FILM (130 degrees C).2) If you laminating thicker glass with more layers of EVA FILM, then the keeping time should belonger, for example if 5mmglass+0.38mm EVA FILM +5mm glass is 130 degree and 40 min, then10mm glass+2layer EVA FILM +10mm glass should be 130 degree and 55mins.Because more time is needed for the heat pass through the thicker glass and more layer of EVAFILM.3) The tempered glass laminating with EVA FILM needs longer keeping time than the flat glasslaminating with EVA FILM.4) If the weather is colder in your region, then the keeping time should be longer.And it’s also different for different glass laminating machine, because the heating part is different.So :1) If you change the EVA FILM supplier, maybe you have to adjusting the processing parametersfor laminating glass with EVA FILM.2) If you buy a new EVA glass laminating machine, and the processing parameters maybedifferent from your older one.
3) If the weather changes from different seasons, maybe you also need to adjust the processingparameters for laminating glass with EVA FILM.4) Yes, every EVA FILM Manufacturers would offer you the processing instructions or parametersfor laminating glass with EVA FILM, but you don’t have to follow them exactly. You should changesome according to your real situation.Why Two Periods of Temperature for Laminating Glass with EVA FILM?1)Low temperature period can help vacuuming, at this temperature the EVA Film is still notmelted, but the temperature is higher than room temperature, the numerators of air would movefaster, which is helpful for the vacuuming. If vacuuming is not good, the bubbles would come outthe laminated glass.2)If the moisture in your place is high, and maybe the EVA FILM has already absorbed somemoisture, the low temperature period would help dry the EVA FILM before the EVA FILM start tomelt, which can avoid bubbles and be good for the adhesion of the EVA FILM.3)If you wash the glass, and maybe the glasses are not dry enough, the low temperature periodcan help dry the glasses.For laminating with papers, if you print ink in the papers are not dry enough, the low temperatureperiod can help dry the print ink.4)And also, after the low temperature period, the machine is stay hot too, so temperaturedetector can measure a more correct temperature closer to real temperature of the laminatedglass.Notes of Making Laminated Glass with EVA Interlayer Film1).Glass is not a good conductor of heat, so please dont laminate different thickness of glassesat the same silicone bag. Its more easily for the thin laminated glass with EVA Interlayer Film totransfer heat, so the keeping heating time at high temperature can be shorter. And if thelaminated glass is thicker, the keeping heating time for the high temperature should be longer.2).For the different thickness of the fabric or papers, the thickness of EVA interlayer film shouldbe different. For the thin and small silk, the 0.25 thickness EVA interlayer film would be OK. Forthe thicker and bigger silk or fabric, the thickness of EVA Interlayer Film should be 0.38mm ormore.3).Normally, the EVA Interlayer Film is soften at 75 degree C and start to react at about 100
degree C. And the EVA Interlayer Film would be totally melted at about 115 degree C. Generallyspeaking, when the detector gets the temperature of 120degree C, the real temperature of EVAInterlayer Film gets 115 degree C.4).The mobility of different thickness of EVA Interlayer Films is different when being heated. Themobility of thicker EVA Interlayer Film is more than the thinner EVA Interlayer Film. So pleaseadjust the time of high-temperature-period of different thickness EVA Interlayer Film. If thehigh-temperature-period is too long, the melted EVA Film Interlayer would leak from thelaminated glass, which will cause bubbles in the edges of laminated glass.5).The quality of laminated glass is partly decided by the plainness of the glasses. So please tryto select the good plainness of flat glass. If you are laminating with tempered glass, please usethe thicker EVA Film Interlayer. For the poor plainness glass, the laminated glass may be brokenwhen vacuuming or cause bubbles of laminated glass.All rights reserved by CNC GLASS INTERLAYER TECH:Product 1]CNC-Force EVA INERLAYER FOR ARCHITECTURAL LAMINATED GLASSeva@evafilms.comProduct 2]CNC-SmartSMART FILM FOR PRIVACY SWITCHABLE GLASSsmartfilm@smartestglass.comProduct 3]CNC-Shield PVB INTERLAYER FOR AUTOMOTIVE WINDSHIELD GLASSpvb@pvbfilm.netWeb: www.CNCglass.com www.CNCnext.comMail: firstname.lastname@example.org@gmail.com